Electroluminescence of InGaN/GaN heterostructures
at the reverse bias and nitrogen temperature
VITALY VELESCHUK1*, ALEXANDER VLASENKO1, MAXIM KISSELYUK1, ZOYA VLASENKO1, DENIS KHMIL’1, VLADIMIR BORSHCH2
1V. Lashkaryov Institute of Semiconductor Physics, National Academy of Sciences of Ukraine, 41 Nauki Ave, 03680 Kyiv, Ukraine
2Poltava National Technical Yuri Kondratyuk University, 24 Pershotravnevyi Ave, 36011 Poltava, Ukraine *Corresponding author: firstname.lastname@example.org
The electroluminescence spectra at reverse biases in LED InGaN/GaN heterostructures at liquid nitrogen temperatures were studied. At the reverse bias and T = 77 K, avalanche microplasmas breakdowns were observed. Electroluminescence spectra demonstrate two peaks caused by the recombination of carriers in different parts of the structure (quantum well and p-GaN layer). The temperature narrowing the half-width and the shift of electroluminescence spectra peaks inherent to microplasmas were observed.
Keywords: electroluminescence at reverse bias, InGaN/GaN heterostructures, defect.
To realize the operative non-destructive diagnostics of InGaN/GaN heterostructures as a base for powerful LEDs, the electroluminescence (EL) at the forward bias, photo-and cathode-luminescence (PL, CL) , are used most often. At the same time, the ap-plication of the reverse bias in GaN structures enables to observe an avalanche microplas-ma breakdown that takes place predominantly within the ranges of critical extended defects and is accompanied by luminescence [2–11]. EL spectra at the reverse bias and operation temperatures were investigated in typical LED InGaN/GaN [3–7] and AlGaN/GaN heterostructures  as well as GaNP , ZnO/GaN [10, 11], GaAs  and Si [12, 13] structures.
In addition, some separate and well resolved lines in luminescence spectra, which are observed at lowered temperatures, contain information about the energy levels of recombination centers and defects, including deep levels (DL). From measurements
of temperature dependences typical for luminescence spectra, it becomes possible to determine the temperature coefficients dE/dT, activation energy, etc.
At lowered temperatures, in particular at the liquid nitrogen one, EL spectra at re-verse biases in LED heterostructures InGaN/GaN are not studied well. It is obvious that EL spectra can contain additional information about critical defects, whose influ-ence prevails in characteristics of device structures. Investigation of EL spectra inher-ent to microplasmas (MP) at low temperatures is also important from the viewpoint of predicting the reliability of GaN structures. The study of MP breakdown is not limited by the above problems: for example, MP worsens the characteristics of Zener diodes and photodiodes based on GaN.
2. Experimental details
InxGa1 – xN/GaN structures of powerful LEDs (Pel= 1 W, Inom= 350 mA, the area of heterostructures was close to 1 mm2) with various composition of indium in the quan-tum well (QW) x = 0.2 and 0.3 on Al2O3 substrate were investigated in this work. The colors of emission from these heterostructures were blue and green, respectively. The EL spectra of MP had a very weak intensity and were measured using a spectro-radiometer HAAS-2000 (Everfine) with a long time of integration for clear detection of spectral lines. The time of spectral measurements was 5 or 10 min. For measure-ments in liquid nitrogen, a special cell with the output window was used.
Since the reverse current in LED structures InGaN/GaN at T = 77 K is practically one order lower than that at room temperature, the EL intensity of MP is also lower, being in proportion to the current [3, 4]. Therefore, to detect EL of MP at 77 K, it is necessary to apply higher voltages, which in some cases results in a shunting or cata-strophic breakdown. Some results typical for three samples of LEDs with blue emission and the one with green emission are presented below.
Adduced in Fig. 1 are MP spectra at T = 77 and 300 K for two heterostructures with
x = 0.2. At room temperature, one can see the wideband with the maximum near
2.72 eV (Fig. 1a) and 2.65 eV (Fig. 1b). At liquid nitrogen temperature, one can see already two peaks at 2.80 and 2.65 eV (Fig. 1a) as well as 2.84 and 2.65 eV (Fig. 1b). Some shift of the short-wave wing in the spectrum at T = 77 K due to Eg increasing is also observed.
Figure 2 shows the MP spectra of the structure no. 1 at T = 77 K. These are changed with increasing the current from 1.9 up to 2.2 mA (curves 1 to 3). Besides, one can observe the intensity growth of the band at λ= 469 nm (2.65 eV). The half-width of this band is close to 14 nm (curve 3) at the reverse bias. The half-width of EL spectrum at the forward bias (T = 300 K) is equal to 25 nm (curve 4). The new appearing band in the spectrum 3 is ascribed to EL emission from the quantum well, the half-width of which is lower due to nitrogen temperature. A similar growth of the EL peak related
2.8 eV 2.72 eV 2.65 eV 1 2 1 – T = 77 K, Urev = –50 V, I = 1.9 mA 1.0 0.8 0.6 0.4 0.2 In te nsit y [a . u .] 2 – T = 300 K, Urev = –45 V, I = 3.3 mA a 2.84 eV 2.65 eV 2.65 eV 1 (×0.5) 2 1 – T = 77 K, Urev = –52 V, I = 1.2 mA 1.0 0.8 0.6 0.4 0.2 400 450 500 550 600 650 700 Wavelength [nm] In te nsi ty [a . u .] 2 – T = 300 K, Urev = –45 V, I = 1.1 mA b
Fig. 1. EL spectra of microplasmas at the reverse bias of the In0.2Ga0.8N/GaN structures no. 1 (a) and no. 2 (b). 0.0 2 1.4 1.2 1.0 0.8 0.4 400 450 500 550 600 650 700 Wavelength [nm] In tensit y [a . u.] T = 77 K 0.2
Fig. 2. EL spectra of the In0.2Ga0.8N/GaN structure no. 1 with increasing the current.
0.6 1 3 4 1 – Urev = –50 V, I = 1.9 mA 2 – Urev = –50 V, I = 2.1 mA 3 – Urev = –50 V, I = 2.2 mA T = 300 K 4 – Inom = 350 mA (Uforw)
with the QW Al0.1Ga0.9N at room temperature with increasing the reverse bias (from 6.5 up to 14.3 V) was observed in  for p-i-n AlGaN diode as well as for GaAs
p-n junction .
Contrary to the band peak at 2.65 eV, the intensity of the band at 2.8 eV does not practically grow with current (Fig. 2). Let us consider the diagram in Fig. 3. There takes place the injection and acceleration of electrons from the p-GaN and holes from the n-GaN layer as well as excitation of new carriers (multiplication), then their sep-aration by the field and recombination. There occurs an act of ionization (at the defect), drift in the field (acceleration) and recombination. Besides, due to a very small thick-ness of the InGaN layer, tunneling is available there (Fig. 3). Impact ionization takes place due to this tunneling of electrons from the valence band of the p-GaN into the InGaN layer and further into the n-GaN, and this ionization takes place predominantly in QW and n-GaN layer .
Two peaks in the spectra at T = 77 K correspond to two different transitions. The peak at 2.65 eV corresponds to recombination in QW, while the peak at 2.80–2.84 eV arises due to recombination with participation of the pair deep donor – shallow acceptor MgGa (DAP), see Fig. 3. It is the most probable that the role of this donor is performed by MgN, since the emission energy corresponding to the transition MgN–MgGa is close to 2.87 eV . As the p-GaN layer is doped with magnesium up to the level 1019–1020cm–3, MgN donors arise simultaneously with MgGa acceptors [1, 14]. Also in , the PL band at 2.88 eV in GaN:Mg is related with DAP and N vacancies as donors. In the work , after low-energy electron irradiation of InGaN/GaN structures (when the p-layer is doped with magnesium), there arose the band peaking at 2.8 eV. In addition to the results adduced in Figs. 1 and 2, in Fig. 4 the MP spectrum at
T = 300 K (1) and at T = 77 K (2) of the structure no. 3 is shown. It can be seen that MgN EC 2.84 eV MgGa 2.65 eV Tunneling U rev Si p-GaN n-GaN InGaN EV
the spectra are sharply different here: the spectrum at the nitrogen temperature is nar-row and practically coincides with the spectrum at the forward bias, but is rather shift-ed. This shift is mainly caused by the quantum-confined Stark effect (QCSE) [4, 7], but also the temperature increase of Eg takes place. The shift between the spectra 2
and 3 reaches 21 nm. Besides, one can observe temperature contraction of the spectrum half-width: at the forward bias it is equal to 22 nm (spectrum 3), while at the reverse bias it is only 13 nm (spectrum 2).
In this sample for Urev= –34 V at T = 77 K MP emission was so weak that we could not detect it. After keeping the sample under Urev= –36 V for 10 min, we ob-served the irreversible breakdown, the structure failed. LED no. 3 has a lower voltage for MP switching on, lower value of the breakdown voltage, which along with avail-ability of the band near 400 nm indicates a higher concentration of defects .
It has been ascertained that the EL intensity inherent to MP at room temperature is higher than that at nitrogen temperature.
Let us consider EL spectra of MP observed in the heterostructure In0.3Ga0.7N/GaN possessing green emission. Like to the previous case of the sample no. 3, in this heterostructure at the reverse bias one can observe the narrow band typical for forward bias (Fig. 5). But in this structure, the spectrum for the reverse bias is narrow even at
T = 300 K due to predominant recombination in QW In0.3Ga0.7N and not in the adjacent
GaN layers, since conductivity in the In0.3Ga0.7N layer is higher than that in In0.2Ga0.8N. The spectra for forward and reverse biases are shifted due to the QCSE [4, 7] by 19 nm (Fig. 5, spectra 1 and 3), but the temperature shift of the spectrum 2 relatively to the spectrum 1 is absent. The latter can be presumably explained by S-like behavior of the luminescence peak with temperature changing from 10 up to 300 K .
The half-width of the spectra when applying the reverse voltage is close to 36 nm at 300 K and 25 nm at 77 K, while for Inom it is equal to 42 nm, which is higher than
1 1.0 0.8 0.6 0.4 0.2 400 450 500 550 600 650 Wavelength [nm] 1 – Urev = –26 V, T = 300 K 0.0 In te nsi ty [a . u .] 2 3 2 – Urev = –35 V, T = 77 K 3 – Inom = 350 mA, T = 300 K
that in the structure In0.2Ga0.8N/GaN due to higher disordering and segregation of indium in QW InGaN .
As it can be seen from the reverse current-voltage characteristics inherent to the stud-ied heterostructures (Fig. 6), the current value at T = 77 K is approximately one order lower, which results in “switching off” of the part of MP, and the current passes pre-dominantly via remaining MP.
The sharper slope of current-voltage characteristic (CVC) for LED with green emission comparing to LED with blue emission (Fig. 6) can be explained by the higher concentration of defects, which is caused by the disorder in the InGaN layer related with the enhanced indium content (from x = 0.2 to 0.3) as well as by extended defects . The transport-mechanism of current for the reverse CVC in these structures is known
1 1.0 0.8 0.6 0.4 0.2 450 480 510 570 600 Wavelength [nm] 1 – Urev = –20 V, 0.0 In te nsity [a . u .] 2 3 2 – Urev = –25 V, 3 – Inom = 350 mA, 540
Fig. 5. EL spectra of the In0.3Ga0.7N/GaN structure.
T = 300 K T = 77 K T = 300 K 1 10–3 –35 –30 –25 –20 –15 0 Voltage [V] 1 – In0.2Ga0.8N/GaN, T = 77 K Cu rren t [A] 2 3 2 – In0.2Ga0.8N/GaN, T = 300 K 3 – In0.3Ga0.7N/GaN, T = 77 K 4 10–4 10–5 10–6 10–7 10–8 10–9 10–10 –10 –5 4 – In0.3Ga0.7N/GaN, T = 300 K
Fig. 6. Reverse CVCs of the In0.2Ga0.8N/GaN (1, 2) and In0.3Ga0.7N/GaN (3, 4) heterostructures at
– it is Mott variable-range hopping , and only after reaching some voltage, the CVC dependence becomes linear due to many active MPs .
At room temperatures, various LED GaN structures possess predominantly wide EL spectra under the reverse bias [3–8], which is caused by recombination of carriers on impurities and diverse defects in the layers adjacent to the p-n junction, while the wideband of MP spectra corresponds to recombination of carriers mainly at the exter-nal boundaries of a space charge region .
The availability of two peaks at the nitrogen temperature (Fig. 1) as well as the growth of one of them with increasing the current (Fig. 2) indicate two different recombination areas, namely: quantum well and the adjacent GaN layer with participation of DAPs. It is the most probable that the band peaking at 2.80–2.84 eV in Figs. 1 and 2 corre-sponds to emission from DAP MgGa (acceptor) to MgN (donor) present in the GaN layer
heavily doped with magnesium (up to 1019–1020cm–3).
Using the obtained figures, it was ascertained that those MPs present at T = 300 K were kept at T = 77 K too but some part of them disappeared. Location of MP under these temperatures fully coincides. The appearance of narrow bands instead of the wide ones (Figs. 2, 4, 5) indicates band-to-band carrier recombination only in the QW area, since the spectral look is the same as that for forward bias. When the voltage is in-creased, the conductivity of MP grows, but the amounts of free carriers and respec-tively hot electrons are lower at the nitrogen temperature, and the width of the area where the avalanche ionization current takes place is narrower. Respectively, the re-combination area is localized in QW.
It is known that threading dislocations serve as sources of MPs in these structures [3–5, 7], but at the same time it is also known that the current passes along the In-rich areas, because of higher conductivity. Spatial non-uniformity in distribution of In con-tent inside the InGaN layer relatively to the mean In concon-tent becomes more pronounced with x growth and leads to localization of charge carriers . Inside In-rich layers (x = 0.3), the current passes through the areas enriched with In due to solid solution phase decomposition, bulk and surface In segregation, indium accumulation near various de-fects including dislocations. In the paper , for instance, the model of LED as a set of microdiodes connected in parallel and possessing different amounts of In in QW was considered. Sizes of areas comprised by p-n microjunctions are determined by fluctuations in the In content inside the active layer. The absence of the wide MP spec-trum from the structure with green emission (Fig. 5) indicates recombination of carriers predominantly in QW, in particular due to nanoinclusions enriched with indium . On the other hand, lowering the temperature results in changing ionization param-eters (threshold ionization energy, mean free path, drift velocities of carriers  as well as thermal and electrical conductivities, etc.), which results in the temperature de-pendence of MP parameters.
Third, MP channels contain shallow and deep levels and lowering the temperature leads to their elimination via filling them. If DL remains filled inside a depletion layer (for example at lowered temperatures), it results in changing the breakdown voltage inherent to the p-n junction. Since the part of DL is filled, it also influences the EL spectrum.
As ascertained in this work, typical In0.2Ga0.8N/GaN LEDs that under forward bias possess one band in the blue range, at the reverse bias and T = 77 K demonstrate EL MP spectra with two peaks caused by recombination of carriers in different parts of the structure (QW and p-GaN layer). It enables the additional study of recombination centers in a wider region of the depletion layer where impact ionization near extended critical defects takes place.
We have observed the temperature narrowing of the half-width and the shift of EL spectra peaks inherent to microplasmas. The EL spectrum of MPs in In0.3Ga0.7N/GaN structures at T = 77 K contains one peak, which is caused by higher conductivity of the In0.3Ga0.7N layer.
Acknowledgements – Publications are based on the research provided by the grant support of the State
Fund For Fundamental Research (project F64/49-2015). References
 RESHCHIKOV M.A., MORKOÇ H., Luminescence properties of defects in GaN, Journal of Applied Physics 97(6), 2005, article 061301.
 HSIANG CHEN, YIH-MIN YEH, CHUAN HAO LIAO, CHUN WEI LIN, CHUAN-HAUR KAO, TIEN-CHANG LU,
Optical characterizations and reverse-bias electroluminescence observation for reliability investi-gations of the InGaN light emitting diode, Microelectronic Engineering 101, 2013, pp. 42–46.
 MENEGHINI M., VACCARI S., TRIVELLIN N., DANDAN ZHU, HUMPHREYS C., BUTENDHEICH R., LEIRER C., HAHN B., MENEGHESSO G., ZANONI E., Analysis of defect-related localized emission processes in
InGaN/GaN-based LEDs, IEEE Transactions on Electron Devices 59(5), 2012, pp. 1416–1422.
 MENEGHINI M., TRIVELLIN N., PAVESI M., MANFREDI M., ZEHNDER U., HAHN B., MENEGHESSO G., ZANONI E., Leakage current and reverse-bias luminescence in InGaN-based light-emitting diodes, Applied Physics Letters 95(17), 2009, article 173507.
 CAO X.A., LEBOEUF S.F., KIM K.H., SANDVIK P.M., STOKES E.B., EBONG A., WALKER D., KRETCHMER J., LIN J.Y., Jiang H.X., Investigation of radiative tunneling in GaN/InGaN single quantum well
light-emit-ting diodes, Solid-State Electronics 46(12), 2002, pp. 2291–2294.
 KOVALEV A.N., MANYAKHIN F.I., KUDRYASHOV V.E., TURKIN A.N., YUNOVICH A.É., Impact ionization
luminescence of InGaN/AlGaN/GaN p-n-heterostructures, Semiconductors 32(1), 1998, pp. 54–57.
 VELESCHUK V.P., VLASENKO A.I., VLASENKO Z.K., KISSELYUK M.P., BORSHCH V.V., Non-destructive
control of critical defects and diagnostics of InGaN/GaN heterostructures in power LEDs by using their microplasma characteristics, Materials Research Express 2(5), 2015, article 055902.
 ZHANG S.K., WANG W.B., DABIRAN A.M., OSINSKY A., WOWCHAK A.M., HERTOG B., PLAUT C., CHOW P.P., GUNDRY S., TROUDT E.O., ALFANO R.R., Avalanche breakdown and breakdown luminescence of AlGaN
 KIKAWA J., YOSHIDA S., ITOH Y., Electroluminescence studies under forward and reverse bias
conditions of a nitride-rich GaN1 – xPx SQW structure LED grown by laser-assisted metal-organic chemical vapor deposition, Solid-State Electronics 47(3), 2003, pp. 523–527.
 TI WANG, HAO WU, ZHENG WANG, CHAO CHEN, CHANG LIU, Blue light emission from the
hetero-structured ZnO/InGaN/GaN, Nanoscale Research Letters 8(1), 2013, article 99.
 SADAF J.R., ISRAR M.Q., KISHWAR S., NUR O., WILLANDER M., Forward- and reverse-biased
electro-luminescence behavior of chemically fabricated ZnO nanotubes/GaN interface, Semiconductor
Science and Technology 26(7), 2011, article 075003.
 LAHBABI M., AHAITOUF A., FLIYOU M., ABARKAN E., CHARLES J.-P., BATH A., HOFFMANN A., KERNS S.E., KERNS D.V., Analysis of electroluminescence spectra of silicon and gallium arsenide p-n junctions
in avalanche breakdown, Journal of Applied Physics 95(4), 2004, pp. 1822–1828.
 BOTHE K., RAMSPECK K., HINKEN D., SCHINKE C., SCHMIDT J., HERLUFSEN S., BRENDEL R., BAUER J., WAGNER J.-M., ZAKHAROV N., BREITENSTEIN O., Luminescence emission from forward- and reverse
-biased multicrystalline silicon solar cells, Journal of Applied Physics 106(10), 2009, article 104510.
 TITKOV I.E., ZUBRILOV A.S., DELIMOVA L.A., MASHOVETS D.V., LINIĬCHUK I.A., GREKHOV I.V., White
electroluminescence from ZnO/GaN structures, Semiconductors 41(5), 2007, pp. 564–569.
 GEORGOBIANI A.N., GRUZINTSEV A.N., VOROB’EV M.O., KAISER U., RICHTER W., KHODOS I.I., Fine
structure of the edge ultraviolet luminescence of GaN:Mg films activated in a nitrogen plasma and the electroluminescence of a ZnO-GaN:Mg heterostructure based on these films, Semiconductors
35(6), 2001, pp. 695–699.
 VERGELES P.S., YAKIMOV E.B., Effect of low-energy electron irradiation on the optical properties of
structures containing multiple InGaN/GaN quantum well, Semiconductors 49(2), 2015, pp. 143–148.
 HYUN JEONG, HYEON JUN JEONG, HYE MIN OH, CHANG-HEE HONG, EUN-KYUNG SUH, LERONDEL G., MUN SEOK JEONG, Carrier localization in In-rich InGaN/GaN multiple quantum wells for green
light-emitting diodes, Scientific Reports 5, 2015, article 9373.
 FERDOUS M.S., WANG X., FAIRCHILD M.N., HERSEE S.D., Effect of threading defects on InGaN/GaN
multiple quantum well light emitting diodes, Applied Physics Letters 91(23), 2007, article 231107.
 QIFENG SHAN, MEYAARD D.S., QI DAI, JAEHEE CHO, SCHUBERT E.F., JOONG KON SON, CHEOLSOO SONE,
Transport-mechanism analysis of the reverse leakage current in GaInN light-emitting diodes,
Applied Physics Letters 99(25), 2011, article 253506.
 LEVINSHTEĬN M.E., KOSTAMOVAARA J., VAINSHTEIN S., Breakdown Phenomena in Semiconductors
and Semiconductor Devices, World Scientific, 2005, p. 208.
 NIKIFOROV S., SUSHKOV V., Method for testing the potential degree of degradation of light emitting
diode characteristics, Solid-State Lightning, No. 3, 2011, pp. 10–13.
Received April 8, 2015 in revised form June 5, 2015